#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:41:30 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179419 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/16/4331624.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4331624
loop_
_publ_author_name
'Bo Liu'
'Jin Yang'
'Guo-Cheng Yang'
'Jian-Fang Ma'
_publ_contact_author_address
;
Key Lab of Polyoxometalate Science
Department of Chemistry
Northeast Normal University
Changchun 130024
P.R.China
;
_publ_contact_author_email       jianfangma@yahoo.com.cn
_publ_contact_author_fax         +86-431-85098620
_publ_contact_author_name        'Jian-Fang Ma'
_publ_contact_author_phone       +86-431-85098620
_publ_section_title
;
 Four New Three-Dimensional Polyoxometalate-Based Metal-Organic Frameworks
 Constructed From [Mo6O18(O3AsPh)2]4- Polyoxoanions and Copper(I)-Organic
 Fragments: Syntheses, Structures, Electrochemistry, and Photocatalysis
 Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              84
_journal_page_last               94
_journal_paper_doi               10.1021/ic301257k
_journal_volume                  52
_journal_year                    2013
_chemical_formula_moiety         'C16 H21 As Cu2 Mo3 N6 O12'
_chemical_formula_sum            'C16 H21 As Cu2 Mo3 N6 O12'
_chemical_formula_weight         979.06
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 128.4860(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.4377(2)
_cell_length_b                   19.3351(3)
_cell_length_c                   14.3898(4)
_cell_measurement_reflns_used    6935
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.1667
_cell_measurement_theta_min      3.0149
_cell_volume                     2490.97(10)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0201
_diffrn_reflns_av_sigmaI/netI    0.0353
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            10705
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         3.02
_exptl_absorpt_coefficient_mu    4.542
_exptl_absorpt_correction_T_max  0.5490
_exptl_absorpt_correction_T_min  0.4636
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'CrysAlis (Oxford Diffraction, 2006)'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    2.611
_exptl_crystal_description       block
_exptl_crystal_F_000             1887
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.862
_refine_diff_density_min         -1.067
_refine_diff_density_rms         0.096
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.946
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     361
_refine_ls_number_reflns         5057
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.946
_refine_ls_R_factor_all          0.0309
_refine_ls_R_factor_gt           0.0224
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0253P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0478
_refine_ls_wR_factor_ref         0.0487
_reflns_number_gt                4082
_reflns_number_total             5057
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ic301257k_si_002_4.cif
_cod_data_source_block           4
_cod_original_cell_volume        2490.97(9)
_cod_database_code               4331624
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu -0.08043(5) 0.86882(2) 0.43041(4) 0.03242(11) Uani 1 1 d .
Cu2 Cu 0.38262(5) 0.71498(2) 0.44209(4) 0.03219(11) Uani 1 1 d .
As1 As 0.63847(3) 0.951376(15) 0.61119(3) 0.01568(7) Uani 1 1 d .
Mo1 Mo 0.24460(3) 0.888730(13) 0.44126(2) 0.01867(7) Uani 1 1 d .
Mo2 Mo 0.35150(3) 1.011378(14) 0.63524(3) 0.01854(7) Uani 1 1 d .
Mo3 Mo 0.40350(3) 0.874633(14) 0.31547(2) 0.01997(7) Uani 1 1 d .
C1 C -0.3542(4) 0.83784(17) 0.1791(3) 0.0252(7) Uani 1 1 d .
H1 H -0.3436 0.8765 0.1464 0.030 Uiso 1 1 calc R
C2 C -0.4415(4) 0.74789(17) 0.1952(3) 0.0271(8) Uani 1 1 d .
H2 H -0.5016 0.7100 0.1793 0.033 Uiso 1 1 calc R
C3 C -0.2509(4) 0.73468(18) 0.4183(3) 0.0342(8) Uani 1 1 d .
H3A H -0.2649 0.7655 0.4639 0.041 Uiso 1 1 calc R
H3B H -0.1444 0.7302 0.4603 0.041 Uiso 1 1 calc R
C4 C -0.3138(4) 0.66506(18) 0.4111(3) 0.0326(8) Uani 1 1 d .
H4A H -0.3256 0.6381 0.3489 0.039 Uiso 1 1 calc R
H4B H -0.4116 0.6708 0.3907 0.039 Uiso 1 1 calc R
C5 C -0.2117(4) 0.62643(18) 0.5290(3) 0.0330(8) Uani 1 1 d .
H5A H -0.1132 0.6216 0.5505 0.040 Uiso 1 1 calc R
H5B H -0.2019 0.6528 0.5909 0.040 Uiso 1 1 calc R
C6 C -0.2744(4) 0.55606(18) 0.5194(3) 0.0346(9) Uani 1 1 d .
H6A H -0.2796 0.5299 0.4594 0.042 Uiso 1 1 calc R
H6B H -0.3759 0.5618 0.4917 0.042 Uiso 1 1 calc R
C7 C -0.1885(4) 0.51364(17) 0.6326(3) 0.0302(8) Uani 1 1 d .
H7A H -0.0877 0.5055 0.6604 0.036 Uiso 1 1 calc R
H7B H -0.1825 0.5386 0.6939 0.036 Uiso 1 1 calc R
C8 C -0.2668(4) 0.44570(17) 0.6087(3) 0.0306(8) Uani 1 1 d .
H8A H -0.3687 0.4545 0.5778 0.037 Uiso 1 1 calc R
H8B H -0.2707 0.4209 0.5482 0.037 Uiso 1 1 calc R
C9 C -0.0864(4) 0.41737(17) 0.8267(3) 0.0243(7) Uani 1 1 d .
H9 H -0.0352 0.4592 0.8540 0.029 Uiso 1 1 calc R
C10 C -0.1612(4) 0.31637(18) 0.8169(3) 0.0292(8) Uani 1 1 d .
H10 H -0.1705 0.2728 0.8391 0.035 Uiso 1 1 calc R
C11 C 0.8001(3) 0.89786(15) 0.7338(3) 0.0185(7) Uani 1 1 d .
C12 C 0.8913(4) 0.92362(19) 0.8470(3) 0.0323(8) Uani 1 1 d .
H12 H 0.8697 0.9660 0.8638 0.039 Uiso 1 1 calc R
C13 C 1.0158(4) 0.8865(2) 0.9364(4) 0.0440(10) Uani 1 1 d .
H13 H 1.0782 0.9041 1.0132 0.053 Uiso 1 1 calc R
C14 C 1.0470(4) 0.8237(2) 0.9116(4) 0.0432(10) Uani 1 1 d .
H14 H 1.1308 0.7989 0.9718 0.052 Uiso 1 1 calc R
C15 C 0.9552(4) 0.7973(2) 0.7982(4) 0.0408(10) Uani 1 1 d .
H15 H 0.9771 0.7547 0.7824 0.049 Uiso 1 1 calc R
C16 C 0.8298(4) 0.83380(18) 0.7069(3) 0.0329(8) Uani 1 1 d .
H16 H 0.7674 0.8162 0.6302 0.040 Uiso 1 1 calc R
N1 N -0.4657(3) 0.79203(14) 0.1138(2) 0.0255(6) Uani 1 1 d .
N2 N -0.2614(3) 0.82345(14) 0.2928(2) 0.0248(6) Uani 1 1 d .
N3 N -0.3202(3) 0.76540(13) 0.3017(2) 0.0228(6) Uani 1 1 d .
N4 N -0.1935(3) 0.40234(13) 0.7142(2) 0.0230(6) Uani 1 1 d .
N5 N -0.2432(3) 0.33700(14) 0.7060(3) 0.0279(6) Uani 1 1 d .
N6 N -0.0620(3) 0.36420(14) 0.8958(2) 0.0239(6) Uani 1 1 d .
O1 O 0.0621(2) 0.90147(11) 0.3834(2) 0.0277(5) Uani 1 1 d .
O2 O 0.2709(2) 0.80100(11) 0.4642(2) 0.0283(5) Uani 1 1 d .
O3 O 0.2296(2) 0.89428(11) 0.30291(19) 0.0222(5) Uani 1 1 d .
O4 O 0.4979(2) 0.89760(10) 0.51002(18) 0.0179(5) Uani 1 1 d .
O5 O 0.3457(2) 0.91528(11) 0.60276(19) 0.0213(5) Uani 1 1 d .
O6 O 0.5836(2) 1.00512(10) 0.67140(19) 0.0197(5) Uani 1 1 d .
O7 O 0.1683(2) 1.02705(11) 0.5727(2) 0.0265(5) Uani 1 1 d .
O8 O 0.4385(3) 1.00812(12) 0.7830(2) 0.0323(6) Uani 1 1 d .
O9 O 0.3966(2) 1.10328(10) 0.61733(19) 0.0204(5) Uani 1 1 d .
O10 O 0.3244(3) 0.87651(13) 0.1699(2) 0.0366(6) Uani 1 1 d .
O11 O 0.4258(2) 0.78782(11) 0.3509(2) 0.0301(6) Uani 1 1 d .
O12 O 0.7064(2) 0.99703(10) 0.55224(19) 0.0181(5) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0030 0.0020 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0500 2.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3200 1.2650 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6830 0.6860 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0060 0.0030 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0110 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N6 Cu1 N2 141.41(11) 2_556 .
N6 Cu1 O1 102.59(10) 2_556 .
N2 Cu1 O1 109.47(10) . .
N6 Cu1 O7 94.16(10) 2_556 3_576
N2 Cu1 O7 101.71(10) . 3_576
O1 Cu1 O7 98.31(8) . 3_576
N1 Cu2 N5 145.12(12) 4_676 3_566
N1 Cu2 O11 116.86(10) 4_676 .
N5 Cu2 O11 90.71(10) 3_566 .
N1 Cu2 O2 90.46(10) 4_676 .
N5 Cu2 O2 112.61(10) 3_566 .
O11 Cu2 O2 88.20(8) . .
O4 As1 O6 111.00(9) . .
O4 As1 O12 111.81(10) . .
O6 As1 O12 111.27(9) . .
O4 As1 C11 108.74(12) . .
O6 As1 C11 108.44(12) . .
O12 As1 C11 105.33(11) . .
O1 Mo1 O2 104.47(10) . .
O1 Mo1 O3 101.21(10) . .
O2 Mo1 O3 98.51(10) . .
O1 Mo1 O5 100.62(10) . .
O2 Mo1 O5 97.51(10) . .
O3 Mo1 O5 148.64(9) . .
O1 Mo1 O12 94.28(9) . 3_676
O2 Mo1 O12 160.88(9) . 3_676
O3 Mo1 O12 81.17(8) . 3_676
O5 Mo1 O12 74.99(8) . 3_676
O1 Mo1 O4 167.10(9) . .
O2 Mo1 O4 88.23(8) . .
O3 Mo1 O4 74.18(8) . .
O5 Mo1 O4 79.57(8) . .
O12 Mo1 O4 73.22(7) 3_676 .
O1 Mo1 Mo2 90.34(8) . .
O2 Mo1 Mo2 128.70(8) . .
O3 Mo1 Mo2 126.79(6) . .
O5 Mo1 Mo2 31.20(6) . .
O12 Mo1 Mo2 46.00(5) 3_676 .
O4 Mo1 Mo2 83.26(5) . .
O1 Mo1 Mo3 131.94(8) . .
O2 Mo1 Mo3 86.13(7) . .
O3 Mo1 Mo3 30.93(6) . .
O5 Mo1 Mo3 124.71(6) . .
O12 Mo1 Mo3 84.05(5) 3_676 .
O4 Mo1 Mo3 45.28(5) . .
Mo2 Mo1 Mo3 119.409(10) . .
O8 Mo2 O7 103.64(11) . .
O8 Mo2 O5 100.07(10) . .
O7 Mo2 O5 101.46(10) . .
O8 Mo2 O9 101.92(10) . .
O7 Mo2 O9 96.26(9) . .
O5 Mo2 O9 147.52(8) . .
O8 Mo2 O12 164.26(9) . 3_676
O7 Mo2 O12 91.72(9) . 3_676
O5 Mo2 O12 73.09(8) . 3_676
O9 Mo2 O12 79.42(8) . 3_676
O8 Mo2 O6 91.15(9) . .
O7 Mo2 O6 163.67(9) . .
O5 Mo2 O6 82.37(8) . .
O9 Mo2 O6 73.60(8) . .
O12 Mo2 O6 74.07(7) 3_676 .
O8 Mo2 Mo1 131.27(8) . .
O7 Mo2 Mo1 89.68(8) . .
O5 Mo2 Mo1 31.29(6) . .
O9 Mo2 Mo1 123.27(6) . .
O12 Mo2 Mo1 43.95(5) 3_676 .
O6 Mo2 Mo1 85.58(5) . .
O8 Mo2 Mo3 89.91(8) . 3_676
O7 Mo2 Mo3 126.53(7) . 3_676
O5 Mo2 Mo3 127.08(6) . 3_676
O9 Mo2 Mo3 30.46(6) . 3_676
O12 Mo2 Mo3 83.52(5) 3_676 3_676
O6 Mo2 Mo3 45.29(5) . 3_676
Mo1 Mo2 Mo3 119.228(10) . 3_676
O10 Mo3 O11 104.71(12) . .
O10 Mo3 O9 99.98(10) . 3_676
O11 Mo3 O9 99.13(9) . 3_676
O10 Mo3 O3 98.91(10) . .
O11 Mo3 O3 100.03(9) . .
O9 Mo3 O3 148.60(9) 3_676 .
O10 Mo3 O6 92.13(10) . 3_676
O11 Mo3 O6 162.95(10) . 3_676
O9 Mo3 O6 74.84(8) 3_676 3_676
O3 Mo3 O6 79.62(8) . 3_676
O10 Mo3 O4 167.39(10) . .
O11 Mo3 O4 87.59(9) . .
O9 Mo3 O4 80.46(8) 3_676 .
O3 Mo3 O4 75.75(8) . .
O6 Mo3 O4 75.76(7) 3_676 .
O10 Mo3 Mo2 88.85(8) . 3_676
O11 Mo3 Mo2 129.84(7) . 3_676
O9 Mo3 Mo2 30.75(6) 3_676 3_676
O3 Mo3 Mo2 125.70(6) . 3_676
O6 Mo3 Mo2 46.28(5) 3_676 3_676
O4 Mo3 Mo2 85.26(5) . 3_676
O10 Mo3 Mo1 129.06(8) . .
O11 Mo3 Mo1 87.06(7) . .
O9 Mo3 Mo1 127.35(6) 3_676 .
O3 Mo3 Mo1 30.42(6) . .
O6 Mo3 Mo1 84.33(5) 3_676 .
O4 Mo3 Mo1 47.39(4) . .
Mo2 Mo3 Mo1 121.182(10) 3_676 .
N2 C1 N1 114.3(3) . .
N2 C1 H1 122.8 . .
N1 C1 H1 122.8 . .
N3 C2 N1 110.5(3) . .
N3 C2 H2 124.8 . .
N1 C2 H2 124.8 . .
N3 C3 C4 113.0(3) . .
N3 C3 H3A 109.0 . .
C4 C3 H3A 109.0 . .
N3 C3 H3B 109.0 . .
C4 C3 H3B 109.0 . .
H3A C3 H3B 107.8 . .
C3 C4 C5 111.1(3) . .
C3 C4 H4A 109.4 . .
C5 C4 H4A 109.4 . .
C3 C4 H4B 109.4 . .
C5 C4 H4B 109.4 . .
H4A C4 H4B 108.0 . .
C6 C5 C4 110.4(3) . .
C6 C5 H5A 109.6 . .
C4 C5 H5A 109.6 . .
C6 C5 H5B 109.6 . .
C4 C5 H5B 109.6 . .
H5A C5 H5B 108.1 . .
C5 C6 C7 115.9(3) . .
C5 C6 H6A 108.3 . .
C7 C6 H6A 108.3 . .
C5 C6 H6B 108.3 . .
C7 C6 H6B 108.3 . .
H6A C6 H6B 107.4 . .
C8 C7 C6 109.3(3) . .
C8 C7 H7A 109.8 . .
C6 C7 H7A 109.8 . .
C8 C7 H7B 109.8 . .
C6 C7 H7B 109.8 . .
H7A C7 H7B 108.3 . .
N4 C8 C7 112.9(3) . .
N4 C8 H8A 109.0 . .
C7 C8 H8A 109.0 . .
N4 C8 H8B 109.0 . .
C7 C8 H8B 109.0 . .
H8A C8 H8B 107.8 . .
N4 C9 N6 110.5(3) . .
N4 C9 H9 124.8 . .
N6 C9 H9 124.8 . .
N5 C10 N6 113.9(3) . .
N5 C10 H10 123.1 . .
N6 C10 H10 123.1 . .
C12 C11 C16 120.9(3) . .
C12 C11 As1 119.5(2) . .
C16 C11 As1 119.5(3) . .
C11 C12 C13 119.9(4) . .
C11 C12 H12 120.0 . .
C13 C12 H12 120.0 . .
C14 C13 C12 120.0(4) . .
C14 C13 H13 120.0 . .
C12 C13 H13 120.0 . .
C13 C14 C15 120.4(4) . .
C13 C14 H14 119.8 . .
C15 C14 H14 119.8 . .
C14 C15 C16 120.6(4) . .
C14 C15 H15 119.7 . .
C16 C15 H15 119.7 . .
C15 C16 C11 118.2(4) . .
C15 C16 H16 120.9 . .
C11 C16 H16 120.9 . .
C2 N1 C1 102.7(3) . .
C2 N1 Cu2 127.2(2) . 4_475
C1 N1 Cu2 129.9(2) . 4_475
C1 N2 N3 103.3(3) . .
C1 N2 Cu1 133.5(2) . .
N3 N2 Cu1 123.2(2) . .
C2 N3 N2 109.1(3) . .
C2 N3 C3 130.9(3) . .
N2 N3 C3 119.9(3) . .
C9 N4 N5 109.2(3) . .
C9 N4 C8 130.2(3) . .
N5 N4 C8 120.4(3) . .
C10 N5 N4 103.5(3) . .
C10 N5 Cu2 130.3(2) . 3_566
N4 N5 Cu2 125.6(2) . 3_566
C9 N6 C10 102.9(3) . .
C9 N6 Cu1 122.6(2) . 2_546
C10 N6 Cu1 134.4(2) . 2_546
Mo1 O1 Cu1 135.72(12) . .
Mo1 O2 Cu2 138.95(12) . .
Mo1 O3 Mo3 118.65(11) . .
As1 O4 Mo3 129.13(10) . .
As1 O4 Mo1 130.56(10) . .
Mo3 O4 Mo1 87.33(7) . .
Mo2 O5 Mo1 117.51(10) . .
As1 O6 Mo3 128.70(10) . 3_676
As1 O6 Mo2 129.54(11) . .
Mo3 O6 Mo2 88.43(6) 3_676 .
Mo2 O7 Cu1 123.77(11) . 3_576
Mo3 O9 Mo2 118.79(10) 3_676 .
Mo3 O11 Cu2 139.31(12) . .
As1 O12 Mo1 131.26(10) . 3_676
As1 O12 Mo2 130.06(11) . 3_676
Mo1 O12 Mo2 90.04(7) 3_676 3_676
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 N6 1.961(3) 2_556
Cu1 N2 1.968(3) .
Cu1 O1 2.211(2) .
Cu1 O7 2.238(2) 3_576
Cu2 N1 1.949(3) 4_676
Cu2 N5 1.966(3) 3_566
Cu2 O11 2.181(2) .
Cu2 O2 2.237(2) .
As1 O4 1.695(2) .
As1 O6 1.7033(19) .
As1 O12 1.7100(18) .
As1 C11 1.882(3) .
Mo1 O1 1.717(2) .
Mo1 O2 1.719(2) .
Mo1 O3 1.892(2) .
Mo1 O5 1.912(2) .
Mo1 O12 2.2663(19) 3_676
Mo1 O4 2.4155(18) .
Mo1 Mo2 3.2653(4) .
Mo1 Mo3 3.2785(4) .
Mo2 O8 1.698(2) .
Mo2 O7 1.716(2) .
Mo2 O5 1.907(2) .
Mo2 O9 1.912(2) .
Mo2 O12 2.349(2) 3_676
Mo2 O6 2.3692(19) .
Mo2 Mo3 3.2771(4) 3_676
Mo3 O10 1.688(2) .
Mo3 O11 1.726(2) .
Mo3 O9 1.895(2) 3_676
Mo3 O3 1.9202(19) .
Mo3 O6 2.330(2) 3_676
Mo3 O4 2.332(2) .
Mo3 Mo2 3.2771(4) 3_676
C1 N2 1.312(4) .
C1 N1 1.343(4) .
C1 H1 0.9300 .
C2 N3 1.320(4) .
C2 N1 1.332(4) .
C2 H2 0.9300 .
C3 N3 1.463(4) .
C3 C4 1.499(5) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 C5 1.528(5) .
C4 H4A 0.9700 .
C4 H4B 0.9700 .
C5 C6 1.504(5) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 C7 1.516(5) .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
C7 C8 1.504(5) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 N4 1.458(4) .
C8 H8A 0.9700 .
C8 H8B 0.9700 .
C9 N4 1.318(4) .
C9 N6 1.334(4) .
C9 H9 0.9300 .
C10 N5 1.312(4) .
C10 N6 1.352(4) .
C10 H10 0.9300 .
C11 C12 1.369(5) .
C11 C16 1.401(4) .
C12 C13 1.384(5) .
C12 H12 0.9300 .
C13 C14 1.375(5) .
C13 H13 0.9300 .
C14 C15 1.376(6) .
C14 H14 0.9300 .
C15 C16 1.391(5) .
C15 H15 0.9300 .
C16 H16 0.9300 .
N1 Cu2 1.949(3) 4_475
N2 N3 1.355(4) .
N4 N5 1.360(4) .
N5 Cu2 1.966(3) 3_566
N6 Cu1 1.961(3) 2_546
O6 Mo3 2.330(2) 3_676
O7 Cu1 2.238(2) 3_576
O9 Mo3 1.8954(19) 3_676
O12 Mo1 2.2663(19) 3_676
O12 Mo2 2.349(2) 3_676
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O1 Mo1 Mo2 O8 105.17(13) . .
O2 Mo1 Mo2 O8 -3.79(14) . .
O3 Mo1 Mo2 O8 -150.51(13) . .
O5 Mo1 Mo2 O8 -5.08(15) . .
O12 Mo1 Mo2 O8 -159.20(13) 3_676 .
O4 Mo1 Mo2 O8 -86.06(12) . .
Mo3 Mo1 Mo2 O8 -114.42(10) . .
O1 Mo1 Mo2 O7 -2.82(10) . .
O2 Mo1 Mo2 O7 -111.78(12) . .
O3 Mo1 Mo2 O7 101.50(11) . .
O5 Mo1 Mo2 O7 -113.07(13) . .
O12 Mo1 Mo2 O7 92.81(10) 3_676 .
O4 Mo1 Mo2 O7 165.95(9) . .
Mo3 Mo1 Mo2 O7 137.59(7) . .
O1 Mo1 Mo2 O5 110.24(13) . .
O2 Mo1 Mo2 O5 1.29(14) . .
O3 Mo1 Mo2 O5 -145.44(13) . .
O12 Mo1 Mo2 O5 -154.13(13) 3_676 .
O4 Mo1 Mo2 O5 -80.98(12) . .
Mo3 Mo1 Mo2 O5 -109.34(11) . .
O1 Mo1 Mo2 O9 -100.10(10) . .
O2 Mo1 Mo2 O9 150.94(11) . .
O3 Mo1 Mo2 O9 4.22(10) . .
O5 Mo1 Mo2 O9 149.66(13) . .
O12 Mo1 Mo2 O9 -4.47(10) 3_676 .
O4 Mo1 Mo2 O9 68.67(9) . .
Mo3 Mo1 Mo2 O9 40.31(7) . .
O1 Mo1 Mo2 O12 -95.63(10) . 3_676
O2 Mo1 Mo2 O12 155.41(11) . 3_676
O3 Mo1 Mo2 O12 8.69(10) . 3_676
O5 Mo1 Mo2 O12 154.13(13) . 3_676
O4 Mo1 Mo2 O12 73.14(8) . 3_676
Mo3 Mo1 Mo2 O12 44.78(7) . 3_676
O1 Mo1 Mo2 O6 -167.18(9) . .
O2 Mo1 Mo2 O6 83.87(10) . .
O3 Mo1 Mo2 O6 -62.86(9) . .
O5 Mo1 Mo2 O6 82.58(12) . .
O12 Mo1 Mo2 O6 -71.55(9) 3_676 .
O4 Mo1 Mo2 O6 1.60(7) . .
Mo3 Mo1 Mo2 O6 -26.76(5) . .
O1 Mo1 Mo2 Mo3 -135.58(7) . 3_676
O2 Mo1 Mo2 Mo3 115.46(9) . 3_676
O3 Mo1 Mo2 Mo3 -31.26(8) . 3_676
O5 Mo1 Mo2 Mo3 114.17(11) . 3_676
O12 Mo1 Mo2 Mo3 -39.95(7) 3_676 3_676
O4 Mo1 Mo2 Mo3 33.19(5) . 3_676
Mo3 Mo1 Mo2 Mo3 4.831(18) . 3_676
O1 Mo1 Mo3 O10 -1.33(15) . .
O2 Mo1 Mo3 O10 104.68(14) . .
O3 Mo1 Mo3 O10 -8.99(16) . .
O5 Mo1 Mo3 O10 -158.85(13) . .
O12 Mo1 Mo3 O10 -91.74(12) 3_676 .
O4 Mo1 Mo3 O10 -163.98(13) . .
Mo2 Mo1 Mo3 O10 -122.37(11) . .
O1 Mo1 Mo3 O11 -107.93(13) . .
O2 Mo1 Mo3 O11 -1.92(11) . .
O3 Mo1 Mo3 O11 -115.59(15) . .
O5 Mo1 Mo3 O11 94.54(11) . .
O12 Mo1 Mo3 O11 161.66(10) 3_676 .
O4 Mo1 Mo3 O11 89.42(10) . .
Mo2 Mo1 Mo3 O11 131.02(8) . .
O1 Mo1 Mo3 O9 152.82(13) . 3_676
O2 Mo1 Mo3 O9 -101.17(11) . 3_676
O3 Mo1 Mo3 O9 145.16(15) . 3_676
O5 Mo1 Mo3 O9 -4.71(11) . 3_676
O12 Mo1 Mo3 O9 62.41(9) 3_676 3_676
O4 Mo1 Mo3 O9 -9.83(10) . 3_676
Mo2 Mo1 Mo3 O9 31.78(8) . 3_676
O1 Mo1 Mo3 O3 7.67(16) . .
O2 Mo1 Mo3 O3 113.68(15) . .
O5 Mo1 Mo3 O3 -149.86(14) . .
O12 Mo1 Mo3 O3 -82.75(13) 3_676 .
O4 Mo1 Mo3 O3 -154.98(14) . .
Mo2 Mo1 Mo3 O3 -113.38(12) . .
O1 Mo1 Mo3 O6 86.81(11) . 3_676
O2 Mo1 Mo3 O6 -167.18(9) . 3_676
O3 Mo1 Mo3 O6 79.14(13) . 3_676
O5 Mo1 Mo3 O6 -70.72(9) . 3_676
O12 Mo1 Mo3 O6 -3.61(7) 3_676 3_676
O4 Mo1 Mo3 O6 -75.84(8) . 3_676
Mo2 Mo1 Mo3 O6 -34.24(5) . 3_676
O1 Mo1 Mo3 O4 162.65(12) . .
O2 Mo1 Mo3 O4 -91.34(10) . .
O3 Mo1 Mo3 O4 154.98(14) . .
O5 Mo1 Mo3 O4 5.12(10) . .
O12 Mo1 Mo3 O4 72.23(9) 3_676 .
Mo2 Mo1 Mo3 O4 41.60(7) . .
O1 Mo1 Mo3 Mo2 116.12(10) . 3_676
O2 Mo1 Mo3 Mo2 -137.87(8) . 3_676
O3 Mo1 Mo3 Mo2 108.45(12) . 3_676
O5 Mo1 Mo3 Mo2 -41.41(8) . 3_676
O12 Mo1 Mo3 Mo2 25.70(6) 3_676 3_676
O4 Mo1 Mo3 Mo2 -46.53(7) . 3_676
Mo2 Mo1 Mo3 Mo2 -4.929(19) . 3_676
N3 C3 C4 C5 164.0(3) . .
C3 C4 C5 C6 -178.6(3) . .
C4 C5 C6 C7 -176.6(3) . .
C5 C6 C7 C8 179.0(3) . .
C6 C7 C8 N4 -178.4(3) . .
O4 As1 C11 C12 -148.2(2) . .
O6 As1 C11 C12 -27.4(3) . .
O12 As1 C11 C12 91.9(3) . .
O4 As1 C11 C16 35.1(3) . .
O6 As1 C11 C16 155.9(2) . .
O12 As1 C11 C16 -84.9(2) . .
C16 C11 C12 C13 0.7(5) . .
As1 C11 C12 C13 -176.0(3) . .
C11 C12 C13 C14 -0.4(5) . .
C12 C13 C14 C15 0.0(6) . .
C13 C14 C15 C16 0.2(6) . .
C14 C15 C16 C11 0.0(5) . .
C12 C11 C16 C15 -0.5(5) . .
As1 C11 C16 C15 176.2(2) . .
N3 C2 N1 C1 -1.8(4) . .
N3 C2 N1 Cu2 173.6(2) . 4_475
N2 C1 N1 C2 2.4(4) . .
N2 C1 N1 Cu2 -172.9(2) . 4_475
N1 C1 N2 N3 -2.0(3) . .
N1 C1 N2 Cu1 179.6(2) . .
N6 Cu1 N2 C1 171.8(3) 2_556 .
O1 Cu1 N2 C1 -43.7(3) . .
O7 Cu1 N2 C1 59.5(3) 3_576 .
N6 Cu1 N2 N3 -6.4(3) 2_556 .
O1 Cu1 N2 N3 138.1(2) . .
O7 Cu1 N2 N3 -118.6(2) 3_576 .
N1 C2 N3 N2 0.8(4) . .
N1 C2 N3 C3 178.1(3) . .
C1 N2 N3 C2 0.7(3) . .
Cu1 N2 N3 C2 179.3(2) . .
C1 N2 N3 C3 -177.0(3) . .
Cu1 N2 N3 C3 1.7(4) . .
C4 C3 N3 C2 12.3(5) . .
C4 C3 N3 N2 -170.7(3) . .
N6 C9 N4 N5 -0.3(3) . .
N6 C9 N4 C8 174.0(3) . .
C7 C8 N4 C9 11.4(5) . .
C7 C8 N4 N5 -174.9(3) . .
N6 C10 N5 N4 0.0(4) . .
N6 C10 N5 Cu2 171.0(2) . 3_566
C9 N4 N5 C10 0.1(3) . .
C8 N4 N5 C10 -174.8(3) . .
C9 N4 N5 Cu2 -171.4(2) . 3_566
C8 N4 N5 Cu2 13.7(4) . 3_566
N4 C9 N6 C10 0.2(3) . .
N4 C9 N6 Cu1 -176.1(2) . 2_546
N5 C10 N6 C9 -0.1(4) . .
N5 C10 N6 Cu1 175.5(2) . 2_546
O2 Mo1 O1 Cu1 48.9(2) . .
O3 Mo1 O1 Cu1 150.80(16) . .
O5 Mo1 O1 Cu1 -51.85(19) . .
O12 Mo1 O1 Cu1 -127.36(17) 3_676 .
O4 Mo1 O1 Cu1 -141.5(3) . .
Mo2 Mo1 O1 Cu1 -81.48(17) . .
Mo3 Mo1 O1 Cu1 146.80(12) . .
N6 Cu1 O1 Mo1 32.4(2) 2_556 .
N2 Cu1 O1 Mo1 -125.84(18) . .
O7 Cu1 O1 Mo1 128.55(18) 3_576 .
O1 Mo1 O2 Cu2 138.84(18) . .
O3 Mo1 O2 Cu2 34.8(2) . .
O5 Mo1 O2 Cu2 -118.10(19) . .
O12 Mo1 O2 Cu2 -52.7(4) 3_676 .
O4 Mo1 O2 Cu2 -38.86(19) . .
Mo2 Mo1 O2 Cu2 -118.77(17) . .
Mo3 Mo1 O2 Cu2 6.43(18) . .
N1 Cu2 O2 Mo1 109.3(2) 4_676 .
N5 Cu2 O2 Mo1 -97.6(2) 3_566 .
O11 Cu2 O2 Mo1 -7.5(2) . .
O1 Mo1 O3 Mo3 -174.19(12) . .
O2 Mo1 O3 Mo3 -67.51(13) . .
O5 Mo1 O3 Mo3 52.5(2) . .
O12 Mo1 O3 Mo3 93.15(12) 3_676 .
O4 Mo1 O3 Mo3 18.20(10) . .
Mo2 Mo1 O3 Mo3 86.84(12) . .
O10 Mo3 O3 Mo1 172.94(13) . .
O11 Mo3 O3 Mo1 66.16(14) . .
O9 Mo3 O3 Mo1 -60.6(2) 3_676 .
O6 Mo3 O3 Mo1 -96.52(12) 3_676 .
O4 Mo3 O3 Mo1 -18.73(11) . .
Mo2 Mo3 O3 Mo1 -92.02(11) 3_676 .
O6 As1 O4 Mo3 129.31(12) . .
O12 As1 O4 Mo3 4.41(16) . .
C11 As1 O4 Mo3 -111.47(14) . .
O6 As1 O4 Mo1 1.18(17) . .
O12 As1 O4 Mo1 -123.72(13) . .
C11 As1 O4 Mo1 120.39(14) . .
O10 Mo3 O4 As1 -64.2(5) . .
O11 Mo3 O4 As1 128.52(14) . .
O9 Mo3 O4 As1 28.83(13) 3_676 .
O3 Mo3 O4 As1 -130.49(14) . .
O6 Mo3 O4 As1 -47.81(12) 3_676 .
Mo2 Mo3 O4 As1 -1.79(12) 3_676 .
Mo1 Mo3 O4 As1 -143.26(16) . .
O10 Mo3 O4 Mo1 79.0(4) . .
O11 Mo3 O4 Mo1 -88.22(8) . .
O9 Mo3 O4 Mo1 172.09(8) 3_676 .
O3 Mo3 O4 Mo1 12.76(7) . .
O6 Mo3 O4 Mo1 95.45(7) 3_676 .
Mo2 Mo3 O4 Mo1 141.46(5) 3_676 .
O1 Mo1 O4 As1 58.7(5) . .
O2 Mo1 O4 As1 -131.34(15) . .
O3 Mo1 O4 As1 129.30(15) . .
O5 Mo1 O4 As1 -33.37(14) . .
O12 Mo1 O4 As1 43.95(13) 3_676 .
Mo2 Mo1 O4 As1 -2.03(12) . .
Mo3 Mo1 O4 As1 142.35(17) . .
O1 Mo1 O4 Mo3 -83.7(4) . .
O2 Mo1 O4 Mo3 86.31(9) . .
O3 Mo1 O4 Mo3 -13.06(8) . .
O5 Mo1 O4 Mo3 -175.72(8) . .
O12 Mo1 O4 Mo3 -98.40(7) 3_676 .
Mo2 Mo1 O4 Mo3 -144.38(5) . .
O8 Mo2 O5 Mo1 176.13(11) . .
O7 Mo2 O5 Mo1 69.84(12) . .
O9 Mo2 O5 Mo1 -51.9(2) . .
O12 Mo2 O5 Mo1 -18.46(9) 3_676 .
O6 Mo2 O5 Mo1 -94.05(11) . .
Mo3 Mo2 O5 Mo1 -86.28(11) 3_676 .
O1 Mo1 O5 Mo2 -72.66(12) . .
O2 Mo1 O5 Mo2 -178.99(11) . .
O3 Mo1 O5 Mo2 60.8(2) . .
O12 Mo1 O5 Mo2 18.97(9) 3_676 .
O4 Mo1 O5 Mo2 94.22(11) . .
Mo3 Mo1 O5 Mo2 90.52(10) . .
O4 As1 O6 Mo3 -126.77(13) . 3_676
O12 As1 O6 Mo3 -1.56(17) . 3_676
C11 As1 O6 Mo3 113.84(15) . 3_676
O4 As1 O6 Mo2 1.24(17) . .
O12 As1 O6 Mo2 126.45(13) . .
C11 As1 O6 Mo2 -118.15(15) . .
O8 Mo2 O6 As1 129.23(15) . .
O7 Mo2 O6 As1 -75.6(4) . .
O5 Mo2 O6 As1 29.23(14) . .
O9 Mo2 O6 As1 -128.68(15) . .
O12 Mo2 O6 As1 -45.29(13) 3_676 .
Mo1 Mo2 O6 As1 -2.08(13) . .
Mo3 Mo2 O6 As1 -142.04(17) 3_676 .
O8 Mo2 O6 Mo3 -88.73(9) . 3_676
O7 Mo2 O6 Mo3 66.5(3) . 3_676
O5 Mo2 O6 Mo3 171.27(8) . 3_676
O9 Mo2 O6 Mo3 13.35(8) . 3_676
O12 Mo2 O6 Mo3 96.75(7) 3_676 3_676
Mo1 Mo2 O6 Mo3 139.96(5) . 3_676
O8 Mo2 O7 Cu1 78.06(15) . 3_576
O5 Mo2 O7 Cu1 -178.48(12) . 3_576
O9 Mo2 O7 Cu1 -25.85(14) . 3_576
O12 Mo2 O7 Cu1 -105.39(13) 3_676 3_576
O6 Mo2 O7 Cu1 -76.4(4) . 3_576
Mo1 Mo2 O7 Cu1 -149.30(12) . 3_576
Mo3 Mo2 O7 Cu1 -22.18(17) 3_676 3_576
O8 Mo2 O9 Mo3 68.78(13) . 3_676
O7 Mo2 O9 Mo3 174.18(12) . 3_676
O5 Mo2 O9 Mo3 -62.8(2) . 3_676
O12 Mo2 O9 Mo3 -95.24(11) 3_676 3_676
O6 Mo2 O9 Mo3 -18.89(10) . 3_676
Mo1 Mo2 O9 Mo3 -92.08(12) . 3_676
O10 Mo3 O11 Cu2 -131.88(19) . .
O9 Mo3 O11 Cu2 125.20(19) 3_676 .
O3 Mo3 O11 Cu2 -29.8(2) . .
O6 Mo3 O11 Cu2 57.5(4) 3_676 .
O4 Mo3 O11 Cu2 45.27(19) . .
Mo2 Mo3 O11 Cu2 127.05(15) 3_676 .
Mo1 Mo3 O11 Cu2 -2.17(18) . .
N1 Cu2 O11 Mo3 -85.1(2) 4_676 .
N5 Cu2 O11 Mo3 117.1(2) 3_566 .
O2 Cu2 O11 Mo3 4.5(2) . .
O4 As1 O12 Mo1 131.92(14) . 3_676
O6 As1 O12 Mo1 7.17(18) . 3_676
C11 As1 O12 Mo1 -110.14(16) . 3_676
O4 As1 O12 Mo2 -5.73(16) . 3_676
O6 As1 O12 Mo2 -130.48(13) . 3_676
C11 As1 O12 Mo2 112.21(15) . 3_676
